Electrochemistry Communications 99 (2019) 75–80
Contents lists available at ScienceDirect
Electrochemistry Communications journal homepage: www.elsevier.com/locate/elecom
Electrochemical detection of adenine and guanine using a three-dimensional WS2 nanosheet/graphite microfiber hybrid electrode
Jian Zhanga,b, Dong Hanb, Shu Wangc, Xiaodi Zhangc, Ruiqi Yanga, Yanchen Jia, Xin Yua,
Institute for Advanced Interdisciplinary Research (iAIR), University of Jinan, Jinan 250022, China Université de Lyon, Ecole Centrale de Lyon, UMR CNRS 5270, Institut des Nanotechnologies de Lyon, UMR CNRS 5270, Ecully 69130, France c Beijing Institute of Nanoenergy and Nanosystems, Chinese Academy of Sciences, National Center for Nanoscience and Technology (NCNST), Beijing 100083, China b
Keywords: Graphite microfiber WS2 nanosheets Hybrid electrode Electrocatalytic oxidation Nucleobases biosensors
In this work, a WS2 nanosheet/graphite microfiber hybrid electrode has been fabricated by in situ synthesis of WS2 nanosheets on the surface of graphite microfibers. The WS2 nanosheets possess an excellent electrocatalytic oxidation response towards adenine and guanine that encourages the adsorption of nucleobases and charge transfer at the surface of the microfibers. The WS2 nanosheet/graphite microfiber hybrid electrode shows high sensitivity and selectivity for the detection of adenine and guanine. This hybrid microfiber electrode represents an excellent candidate platform for development of an electrochemical biosensor due to its low cost, flexibility and 3D morphology.
1. Introduction The analysis of nucleobases is critical in the life sciences, especially in the diagnosis of infectious diseases and the study of genetic mutations. They store and transmit biological information and can influence various genetic conditions such as metabolic disorders, blood diseases, vision and hearing loss or neurodegenerative diseases [1,2]. Electrochemical methods are considered to be the most convenient and efficacious techniques for detecting nucleobases because they exhibit excellent sensitivity, give quick results, and are cost effective [3–9]. P. Zuman et al. first reported the electrochemical activity of nucleobases in 1955 . However, nucleobases have a weak direct electron transfer capacity, and exhibit quite weak electrocatalytic oxidation ability. High catalytic potentials can adversely affect detection by electrochemical means [11–13]. Therefore, nanomaterials such as graphene, metal nanoparticles and TiO2 have been employed to modify electrodes in order to improve their electrochemical sensing performance [14–18]. Due to their unique physical and chemical properties, nanomaterials based on 2D layered transition metal dichalcogenides (TMDs) have attracted much attention in recent years, particularly for applications in sensing [19–21]. Tungsten disulfide (WS2) consists of S-W-S sandwiches in a trigonal prism configuration. WS2 nanosheets produced by exfoliation from the bulk material or fabricated via hydrothermal methods have been used in gas sensors and biosensors, among other
applications [22–24]. In particular, the interaction of DNA and nucleotides with TMDs has continued to attract much scientific attention. It has been reported that density function theory (DFT) calculations show that the binding energy between a single nucleotide and MoS2 decreases in the order G > A > C > T. The average binding free energy for different single nucleotides A, T, C, G on the MoS2 surface is about 2.29 kcal/mol . In particular, strategies for detecting DNA using either a single WS2 nanosheet or a few layers of nanosheets have been thoroughly discussed. DNA can be adsorbed onto WS2 via van der Waals forces. WS2 is capable of discriminating between single-stranded DNA and double-stranded DNA, which may prove useful in electrochemical or fluorescent sensors for biomedical applications. It has also been found that nucleobases could be physisorbed onto WS2 due to van der Waals interactions [26,27]. Adsorption of nucleobases on monolayer WS2 changes its photoluminescence emissions, which opens the door for the development of label-free optical sensing approaches for DNA sequencing . To the best of our knowledge, the study of WS2 nanosheets for electrocatalytic oxidation of nucleobases has not yet been reported, although layered WS2 nanosheets have been widely studied as electrocatalysts due to their large surface area and excellent electron transfer processes compared to other inorganic nanomaterials [24,25]. TMD catalysts are commonly supported on carbon materials (e.g. carbon nanofibers, carbon nanotubes, graphene, mesoporous carbon, carbon foam) [29–34]. L. Wang et al. synthesized 3D carbon foam
Corresponding author. E-mail address: [email protected]
https://doi.org/10.1016/j.elecom.2019.01.007 Received 21 November 2018; Received in revised form 11 January 2019; Accepted 11 January 2019 Available online 12 January 2019 1388-2481/ © 2019 The Authors. Published by Elsevier B.V. This is an open access article under the CC BY-NC-ND license (http://creativecommons.org/licenses/BY-NC-ND/4.0/).
Electrochemistry Communications 99 (2019) 75–80
J. Zhang et al.
electrodes coated with MoxW1−xS2 alloys with different Mo/W ratios. The electrocatalytic activity towards the hydrogen evolution reaction (HER) can be tuned by varying the ratio of transition metals in the compounds . B. Seo et al. investigated the growth of TMDs (WS2, MoS2) on carbon surfaces inside confined nanopores. Experimental studies and adhesion energy calculations suggested that WS2 and MoS2 favour basal and edge bonding modes with the carbon support, respectively . The electrochemical activity and catalytic properties may vary depending on the energy of adhesion between the TMDs and the various supports . Graphite microfibers have attracted much attention due to their unique 1D fibrous morphology and high electronic conductivity. Small flexible fiber electrodes can potentially be used in vivo. Furthermore, instead of relying on physical adsorption of nanomaterials on glassy carbon, gold or other solid electrodes, nanostructures can be synthesized in situ on the surface of the microfibers, resulting in a larger electrochemically active surface area, higher utilization efficiency, superior electron transfer and excellent stability. Electrochemical biosensors based on nanostructured hybrid microfiber electrodes have been developed for DNA, glucose and H2O2 detection [35–37]. In this work, we have produced WS2 nanosheets in situ on graphite microfibers via a hydrothermal method and obtained a WS2 nanosheet/ graphite microfiber hybrid material. The resulting WS2 nanosheet/ graphite microfiber electrode combines the electronic conductivity and fibrous morphology of graphite fibers with the high electrocatalytic ability of WS2, and has been used as the working electrode in the electrocatalytic oxidation of adenine and guanine. It is assumed that the WS2 nanosheets play an important role in the enhanced charge transfer process and surface adsorption of nucleobases. The fibrous WS2 nanosheet hybrid electrode is considered to be a promising candidate for detection of nucleic acids in in vivo diagnosis and molecular biology research.
and transmission electron microscope (TEM) (JEM 2100F, Japan). The composition of the WS2 nanosheet/graphite fiber hybrid was analysed by an energy-dispersion spectroscope (EDS, Oxford link system), which was equipped with SEM. Raman spectroscopy was carried out using the 532 nm excitation line (LabRAM HR Evolution, HORIBA). X-ray photoelectron spectra (XPS) were recorded using a K-alpha, Thermo Fisher Scientific (ESCALAB 250xi). 2.4. Electrochemical measurements Electrochemical measurements were recorded on a Gamry electrochemical workstation (Gamry Reference 3000, America). A standard three-electrode system was used: Ag/AgCl (saturated KCl) was used as the reference electrode; a Pt plate (1 cm × 1 cm) was used as the counter electrode; the WS2 nanosheet/graphite microfiber material was used as the working electrode. The enrichment of adenine and guanine was performed at the open circuit and the optimal enrichment time at the electrodes was found to be 150 s. 3. Results and discussion The XRD patterns of the WS2 nanosheet/graphite microfiber hybrid were recorded and compared with those of the bare graphite microfiber and WS2 separately (Fig. 1A). The diffraction peak of the graphite microfiber (curve b) centered at 2θ = 25.7 can be assigned to graphite (JCPDS 65-6212). The JPCDS card of WS2 (denoted as a) showed peaks at 14.1°, 33.0°, 58.2° corresponding to (002), (100), and (110) planes, indicating the presence of the WS2 hexagonal phase. The XRD pattern of the crystalline phase of the WS2 nanosheet/graphite microfiber hybrid is given in curve c. Apart from the peak at 14.1°, no other new peaks were observed in the XRD pattern, showing that the nanosheets grow in the (002) direction. The crystalline structure of the WS2 nanosheet/ graphite microfiber hybrid was further characterized using Raman spectroscopy (Fig. 1B). The Raman spectrum of the graphite fiber (curve a) showed typical G and D peaks at 1585 cm−1 and 1350 cm−1, respectively. The Raman spectrum of the WS2 nanosheet/graphite microfiber hybrid also showed peaks at 350 cm−1 and 413 cm−1, which correspond to the E2g and A1g peaks for WS2 (curve b) . The pure graphite microfiber and the WS2 nanosheet/graphite microfiber hybrid were also examined using SEM to check the surface morphology. The graphite microfibers are about 5 μm in diameter and have a smooth surface (Fig. 1C). The image of the WS2 nanosheet/graphite microfiber hybrid shows that the graphite microfiber is buried in dense layers of WS2 nanosheets (Fig. 1D, E). The WS2 nanosheets are randomly connected with each other, forming a porous surface (Fig. 1F). WS2 nanosheets were exfoliated from the surface of the microfibers and characterized using TEM. The TEM images show that the vertical edges of the WS2 nanosheets possess a layered structure (Fig. 1G). Furthermore, the interplanar distance between the lattice fringes was about 0.62 nm, corresponding to the distance between the (002) planes of WS2 crystals (Fig. 1H) . The chemical composition of the WS2/ graphite microfiber hybrid was analysed by energy-dispersion spectroscopy (EDS). The EDS spectrum is shown in Fig. 1I. The elements S, C, O, W and Al were detected, which indicated that the WS2 nanosheet/ graphite microfiber hybrid electrode had been fabricated successfully (Al and O are from the substrate). The molar ratio W:S was calculated to be 5.69:11.98 (which is approximately 1:2) from the peak intensities (see insert in Fig. 1I), confirming the stoichiometry of the product. It is well known that WS2 monosheets can form not only the usual semiconducting prismatic structure (2H-WS2) but also the less common distorted octahedral structure (1T-WS2), which exhibits metallic behavior . The 1T-WS2 form has recently been shown to be very efficient in redox reactions . The chemical composition of the as-prepared WS2 nanosheets on the graphite fiber was further analysed by X-ray photoelectron spectroscopy (XPS). Fig. 2A shows two peaks at 32.0 eV and 34.1 eV for W4f7/2 and W4f5/2 of 1T-WS2, respectively. The
2. Experimental 2.1. Reagents and materials All the reagents used here are commercially available and of analytical grade. WCl6 and thioacetamide (C2H5NS) were bought from Sigma. Adenine and guanine were obtained from Aladdin (Shanghai, China). Phosphate buffer solutions (PBS, 0.1 M) were prepared using Na2HPO4 and NaH2PO4 and were adjusted to pH 7.0. Commercial graphite microfibers were obtained from Toray (M40-JB-12K) (Japan). 2.2. Preparation of WS2 nanosheet/graphite microfiber hybrid material The surfaces of the graphite microfibers were first cleaned by sonicating sequentially in acetone, 3.0 M HNO3, 1.0 M KOH and distilled water for several minutes, followed by drying at 60 °C overnight . In a typical experiment, WS2 nanosheets were then formed on the graphite microfibers through a hydrothermal method . 3 mM WCl6 and 15 mM C2H5NS were dissolved in 50 mL DI water and stirred at room temperature for 60 min. This solution and about 10 cm graphite microfibers were then transferred to a 50 mL Teflon-lined autoclave and heated to 265 °C and kept for 24 h. After cooling to room temperature, the hybrid graphite fibers were washed using DI water, and dried at 50 °C for 6 h, producing the WS2 nanosheet/graphite microfiber hybrid material. 2.3. Materials characterization The crystalline structure of the WS2 nanosheet/graphite microfiber hybrid was obtained with an X-ray diffraction (XRD) spectrometer (D8advance, Bruker AXS, Germany). The morphology of the WS2 nanosheet/graphite microfiber hybrid was characterized by a field emission scanning electron microscope (FESEM) (HITACHI S8020, Japan) 76
Electrochemistry Communications 99 (2019) 75–80
J. Zhang et al.
Fig. 1. (A) XRD patterns of (a) WS2 (JCPDS 84-1398), (b) graphite microfiber (JCPDS 65–6212) and (c) WS2 nanosheet/graphite microfiber. (B) Raman spectra of (a) graphite microfiber and (b) WS2 nanosheet/graphite microfiber hybrid. SEM images of (C) graphite microfiber, (D, E) WS2 nanosheet/graphite microfiber hybrid and (F) high resolution SEM image of WS2 nanosheets. (G, H) TEM images of WS2 nanosheets. (I) EDS spectrum of WS2 nanosheet/graphite microfiber on Al substrate.
characteristic peaks of 2H-WS2 are shifted by about 0.9 eV to a higher binding energy compared to those of 1T-WS2, being located at 32.9 eV and 35.0 eV, respectively. In addition, WS2 is partially oxidized, as evidenced by the characteristic peaks of W6+ at 36.0 eV and 38.1 eV. Fig. 2B shows the high-resolution XPS S2p spectrum. Two peaks are located at 161.8 eV and 163.5 eV, corresponding to the S2p3/2 and S2p1/2 of 1T-WS2, respectively. Similarly, it is found that the S2p peaks of 2H-WS2 are shifted to a higher bonding energy compared with those of 1T-WS2. The 1T-WS2 and 2H-WS2 coexist in the sample with a ratio of 2.5/1 (1 T/2H) [31,44]. Furthermore, the composition after the electrochemical oxidative treatment was also investigated. As shown in Fig. 2C and D, the XPS peaks show no obvious change compared with those recorded before the electrochemical oxidative treatment, indicating that the WS2 nanosheet/graphite microfiber hybrid electrode has excellent stability. The electrocatalytic oxidation of adenine and guanine at the WS2 nanosheet/graphite microfiber electrode was explored by cyclic voltammetry (CV). Fig. 3A shows the CVs recorded at a graphite microfiber electrode and a WS2 nanosheet/graphite microfiber electrode in 0.1 M PBS at pH 7.0 containing 1 × 10−5 M adenine and 1 × 10−5 M guanine at a scan rate of 100 mV s−1. At the graphite microfiber electrode, two broad oxidation peaks were observed at +0.73 and + 1.03 V, corresponding to the electrochemical oxidation of adenine and guanine, respectively. However, two well-defined oxidation peaks for adenine and guanine were observed when using the WS2 nanosheet/graphite
microfiber electrodes. Note that these two peak potentials are about 90 mV and 70 mV more negative than those at the graphite microfiber electrode, indicating the catalytic activity of the WS2 nanosheets towards the oxidation of adenine and guanine. In addition, the peaks with higher currents at the WS2 nanosheet/graphite microfiber electrode are much sharper than those at the graphite microfiber electrode, indicating the good electrocatalytic oxidation behaviour of WS2 nanosheets towards adenine and guanine. The highly electrocatalytic activity of the WS2 nanosheet/graphite microfiber electrode may be due to the layered WS2 nanosheets increasing the surface area of the microfiber electrode and promoting electron transfer. The CVs of adenine and guanine at the WS2 nanosheet/graphite microfiber electrode were then recorded at various scan rates (Fig. 3B). The oxidation peak currents increase linearly with the scan rate from 50 mV s−1 to 300 mV s−1, which suggests that the electrocatalytic oxidation of adenine and guanine at the WS2 nanosheet/graphite microfiber electrode is a surface-controlled process (Fig. 3C) . The electron transfer kinetics and electrocatalytic ability of transition metal dichalconides can be improved using carbon supports or electrochemical treatments. X. Chia et al. demonstrated an electrochemical method to alter the electron transfer kinetics and catalytic properties of MoS2 films, in which a 2H-1T transition was observed on applying an electrochemical potential. We therefore investigated the composition of the WS2 nanosheets after the electrochemical detection of adenine and guanine. High-resolution XPS spectra recorded in the 77
Electrochemistry Communications 99 (2019) 75–80
J. Zhang et al.
Fig. 2. High-resolution XPS W4f and S2p spectra of as-prepared WS2 nanosheet/graphite microfiber (A, B) and after the electrochemical detection of adenine and guanine (C, D).
W4f and S2p regions are shown in Fig. 2C and D. From the XPS results, it is evident that the surface chemistry remains practically unaltered during the electrochemical treatments, which suggests that the variation in electrocatalytic behaviour is caused by electronic changes rather than surface changes . Electrochemical treatment of the WS2 nanosheets/graphite microfiber electrode may be a good topic for future research. Fig. 4A displays the differential pulse voltammograms (DPV) of 2 × 10−5 M adenine and 2 × 10−5 M guanine in 0.1 M PBS solution (pH 7.0). The DPV peak potential of guanine at a graphite microfiber electrode is located at 0.75 V. In the case of the WS2 nanosheet/graphite microfiber electrode, the peak potential is negatively shifted to 0.66 V. For adenine, the oxidation peak potential on WS2 nanosheet/graphite microfiber electrodes is also negatively shifted to 0.96 V. Compared to the current response of a bare graphite microfiber electrode (curve c), the oxidation peak currents of adenine and guanine obtained at a WS2 nanosheet/graphite microfiber electrode (curve d) are obviously higher. The enhancement in the peak current and the negative shift of
the oxidation potential are clear evidence of the electrocatalytic activity of WS2 nanosheets towards the oxidation of guanine and adenine. The determination of adenine and guanine at a WS2 nanosheet/ graphite microfiber electrode was explored by DPV. The peak currents increased with the increasing concentration of adenine and guanine (Fig. 4B). Fig. 4C shows the linear relationship between the peak currents and the concentration of adenine and guanine. A good linear response to either adenine or guanine concentrations is obtained within the range from 0.5 μM to 20 μM (correlation coefficient 0.993). The detection limits based on S/N = 3 for adenine and guanine were calculated to be 5 × 10−8 M and 9 × 10−8 M, respectively. The proposed WS2 nanosheet/graphite microfiber electrode may therefore be used for the sensitive determination of adenine and guanine. The effect of interfering species was investigated by adding different types of ions into the PBS containing 2 × 10−5 M adenine and 2 × 10−5 M guanine (Fig. 4D). It can be seen that inorganic ions such as Mg2+, Ca2+, Zn2+, Cl−, NO3− and SO42− had almost no effect on the determination of guanine and adenine (signal change < 5.0%).
Fig.3. (A) CV of 0.1 M PBS (pH 7.0) without guanine and adenine at the graphite microfiber electrode (curve a) and WS2 nanosheet/graphite microfiber electrode (curve b). CV of 0.1 M PBS (pH 7.0) with 1 × 10−5 M guanine and adenine at the graphite microfiber electrode (curve c) and WS2 nanosheet/graphite microfiber electrode (curve d) (scan rate 100 mV s−1). (B) CV of 0.1 M PBS (pH 7.0) with 1 × 10−5 M guanine and adenine at the WS2 nanosheet/graphite microfiber electrode at different scan rates; (C) variation of peak currents with potential scan rates. 78
Electrochemistry Communications 99 (2019) 75–80
J. Zhang et al.
Fig. 4. (A) DPV of 0.1 M PBS (pH 7.0) without guanine and adenine at a graphite microfiber electrode (curve a) and a WS2 nanosheet/graphite microfiber electrode (curve b). DPV of 0.1 M PBS (pH 7.0) with 2 × 10−5 M adenine and 2 × 10−5 M guanine at a graphite microfiber electrode (curve c) and a WS2 nanosheet/ graphite microfiber electrodes (curve d). (B) DPV of guanine and adenine in 0.1 M PBS (pH 7.0) at a WS2 nanosheet/graphite microfiber electrode with the concentration ranging from 0.5 to 20 μM. (C) Calibration plots of the peak currents versus the concentration of guanine and adenine. (D) The influence of some ions and important biological substances on the peak currents of adenine and guanine in 0.1 M PBS (pH 7.0) at the WS2 nanosheet/graphite microfiber electrode.
The long-term stability of the WS2 nanosheet/graphite microfiber electrodes was also investigated. These electrodes retained 93% of their initial current response after 2 weeks stored in pH 7.0 PBS at 4 °C, demonstrating that the microfiber electrode retains an acceptable detection performance for a reasonable time.
nanoplates and modifier, Mater. Sci. Eng. C 69 (2016) 128–133.  H. Beitollahi, F. Ebadinejad, F. Shojaie, M. Torkzadeh-Mahani, A magnetic core–shell [email protected]
/MWCNT nanocomposite modified carbon paste electrode for amplified electrochemical sensing of amlodipine and hydrochlorothiazide, Anal. Methods 8 (2016) 6185–6193.  H. Beitollahi, A. Gholami, M.R. Ganjali, Preparation, characterization and electrochemical application of Ag–ZnO nanoplates for voltammetric determination of glutathione and tryptophan using modified carbon paste electrode, Mater. Sci. Eng. C 57 (2015) 107–112.  S. Zhong, J. Zhuang, D. Yang, D. Tang, Eggshell membrane-templated synthesis of 3D hierarchical porous Au networks for electrochemical nonenzymatic glucose sensor, Biosens. Bioelectron. 96 (2017) 26–32.  H. Cao, D. Yang, D. Ye, X. Zhang, X. Fang, S. Zhang, B. Liu, J. Kong, Protein-inorganic hybrid nanoflowers as ultrasensitive electrochemical cytosensing interfaces for evaluation of cell surface sialic acid, Biosens. Bioelectron. 68 (2015) 329–335.  C. Hu, D. Yang, F. Zhu, F. Jiang, S. Shen, J. Zhang, Enzyme-labeled [email protected]
nanocomposite as a facile electrochemical biosensing interface for sensitive glucose determination, ACS Appl. Mater. Interfaces 6 (2014) 4170–4178.  C. Hu, D. Yang, Z. Wang, L. Yu, J. Zhang, D. Cui, N. Jia, Improved EIS performances of an electrochemical cytosensor using three-dimensional architecture [email protected]
as sensing layer, Anal. Chem. 85 (2013) 5200–5206.  O. Manousek, P. Zuman, Polarographie der Harnstoff- und Thioharnstoffderivate V. Anodische depolarisation in Lösungen von Uracil, seiner Derivate und 4-Methyl-2thiouracil, Collect. Czechoslov. Chem. Commun. 20 (1955) 1340–1352.  L. Trnková, J. Friml, O. Dračka, Elimination voltammetry of adenine and cytosine mixtures, Bioelectrochemistry 54 (2001) 131–136.  M. Fojta, L. Havran, R. Kizek, S. Billova, E. Palecek, Multiply osmium-labeled reporter probes for electrochemical DNA hybridization assays: detection of trinucleotide repeats, Biosens. Bioelectron. 20 (2004) 985–994.  Y. Fan, K. Huang, D. Niu, C. Yang, Q. Jing, TiO2-graphene nanocomposite for electrochemical sensing of adenine and guanine, Electrochim. Acta 56 (2011) 4685–4690.  J. Cui, D. Sun, W. Zhou, H. Liu, P. Hu, N. Ren, H. Qin, Z. Huang, J. Lin, H. Ma, Electrocatalytic oxidation of nucleobases by TiO2 nanobelts, Phys. Chem. Chem. Phys. 13 (2011) 9232–9237.  T. Yang, Q. Guan, Q. Li, L. Meng, L. Wang, C. Liu, K. Jiao, Large-area, three-dimensional interconnected graphene oxide intercalated with self-doped polyaniline nanofibers as a free-standing electrocatalytic platform for adenine and guanine, J. Mater. Chem. B 1 (2013) 2926–2933.  T. Yang, M. Chen, F. Nan, L. Chen, X. Luo, K. Jiao, Enhanced electropolymerization of poly(xanthurenic acid)–MoS2 film for specific electrocatalytic detection of guanine and adenine, J. Mater. Chem. B 3 (2015) 4884–4891.  H. Maleh, A. Bananezhad, M. Ganjali, P. Norouzi, A. Sadrnia, Surface amplification of pencil graphite electrode with polypyrrole and reduced graphene oxide for fabrication of a guanine/adenine DNA based electrochemical biosensors for determination of didanosine anticancer drug, Appl. Surf. Sci. 441 (2018) 55–60.  F. Xiao, F. Zhao, J. Li, L. Liu, B. Zeng, Characterization of hydrophobic ionic liquidcarbon nanotubes–gold nanoparticles composite film coated electrode and the simultaneous voltammetric determination of guanine and adenine, Electrochim. Acta
4. Conclusions In this work, WS2 nanosheets were successfully prepared in situ on the surface of graphite microfibers to form a hybrid WS2 nanosheet/ graphite microfiber material, which was used as the working electrode for electrocatalytic oxidation of adenine and guanine. The WS2 nanosheet/graphite microfiber electrode exhibits good electrocatalytic oxidation activity towards adenine and guanine due to its good adsorption ability and the charge transfer provided by the WS2 nanosheets. The hybrid WS2 nanosheet/graphite microfiber electrode could detect adenine and guanine with high sensitivity, high selectivity and good stability. Furthermore, because of its fiber morphology and flexibility, the electrode has the potential to monitor nucleobases in some difficult environments, even within a targeted cell or in vivo. We believe that this hybrid WS2 nanosheet/graphite microfiber electrode offers a significant new platform for biosensing applications. Acknowledgments The work was supported by the Major Program of Shandong Province Natural Science Foundation (No. ZR2018ZC0843), Natural Science Foundation of Shandong Province (No. ZR2018BEM010), the National Natural Science Foundation of China (No. 51802115). References  O. Pänke, A. Kirbs, F. Lisdat, Voltammetric detection of single base-pair mismatches and quantification of label-free target ssDNA using a competitive binding assay, Biosens. Bioelectron. 22 (2007) 2656–2662.  J. Wang, Electrochemical nucleic acid biosensors, Anal. Chim. Acta 469 (2002) 63–71.  H. Beitollahi, S.G. Ivari, M. Torkzadeh-Mahani, Voltammetric determination of 6thioguanine and folic acid using a carbon paste electrode modified with ZnO-CuO
Electrochemistry Communications 99 (2019) 75–80
J. Zhang et al. 53 (2008) 7781–7788.  X. Huang, Z. Zeng, H. Zhang, Metal dichalcogenide nanosheets: preparation, properties and applications, Chem. Soc. Rev. 42 (2013) 1934–1946.  P.K. Kannan, D.J. Late, H. Morgan, C.S. Rout, Recent developments in 2D layered inorganic nanomaterials for sensing, Nanoscale 7 (2015) 13293–13312.  Q. Lu, Y. Yu, Q. Ma, B. Chen, H. Zhang, 2D transition-metal-dichalcogenide-nanosheet-based composites for photocatalytic and electrocatalytic hydrogen evolution reactions, Adv. Mater. 28 (2016) 1917–1933.  A. Li, J. Zhang, J. Qiu, Z. Zhao, C. Wang, C. Zhao, H. Liu, A novel aptameric biosensor based on the self-assembled DNA–WS2 nanosheet architecture, Talanta 163 (2017) 78–84.  S. Wang, Y. Zhang, Y. Ning, G. Zhang, A WS2 nanosheet-based platform for fluorescent DNA detection via PNA–DNA hybridization, Analyst 140 (2015) 434–439.  W. Yan, A.H. Trochimczyk, H. Long, L. Chan, T. Pham, M. Hu, Y. Qin, A. Zettl, C. Carraro, M.A. Worsley, R. Maboudian, Conductometric gas sensing behavior of WS2 aerogel, FlatChem 5 (2017) 1–8.  L. Liang, W. Hu, Z. Xue, J.W. Shen, Theoretical study on the interaction of nucleotides on two-dimensional atomically thin graphene and molybdenum disulfide, FlatChem 2 (2017) 8–14.  C. Lu, Y. Liu, Y. Ying, J. Liu, Comparison of MoS2, WS2, and graphene oxide for DNA adsorption and sensing, Langmuir 33 (2017) 630–637.  H. Vovusha, B. Sanyal, Adsorption of nucleobases on 2D transition-metal dichalcogenides and graphene sheet: a first principles density functional theory study, RSC Adv. 5 (2015) 67427–67434.  S. Feng, C. Cong, N. Peimyoo, Y. Chen, J. Shang, C. Zou, B. Cao, L. Wu, J. Zhang, M. Eginligil, X. Wang, Q. Xiong, A. Ananthanarayanan, P. Chen, B. Zhang, T. Yu, Tunable excitonic emission of monolayer WS2 for the optical detection of DNA nucleobases, Nano Res. 11 (2018) 1744–1754.  C. Zhu, X. Mu, P.A. van Aken, Y. Yu, J. Maier, Single-layered ultrasmall nanoplates of MoS2 embedded in carbon nanofibers with excellent electrochemical performance for lithium and sodium storage, Angew. Chem. Int. Ed. 126 (2014) 2184–2188.  M. Piao, C. Li, M.K. Joo, J. Chu, X. Wang, Y. Chi, H. Zhang, H. Shi, Hydrothermal synthesis of stable 1T-WS2 and single-walled carbon nanotube hybrid flexible thin films with enhanced thermoelectric performance, Energ. Technol. 6 (2018) 1921–1928.  L. Wang, Z. Sofer, J. Luxa, M. Pumera, MoxW1−xS2 solid solutions as 3D electrodes for hydrogen evolution reaction, Adv. Mater. Interfaces 2 (2015) 1500041.  B. Seo, G.Y. Jung, J.H. Kim, T.J. Shin, H.Y. Jeong, S.K. Kwak, S.H. Joo, Preferential
            
horizontal growth of tungsten sulfide on carbon and insight into active sulfur site for the hydrogen evolution reaction, Nanoscale 10 (2018) 3838–3848. X. Zheng, J. Xu, K. Yan, H. Wang, Z. Wang, S. Yang, Space-confined growth of MoS2 nanosheets within graphite: the layered hybrid of MoS2 and graphene as an active catalyst for hydrogen evolution reaction, Chem. Mater. 26 (2014) 2344–2353. C. Tsai, F. Abild-Pedersen, J.K. Nørskov, Tuning the MoS2 edge-site activity for hydrogen evolution via support interactions, Nano Lett. 14 (2014) 1381–1387. J. Zhang, X. Yu, W. Guo, J. Qiu, X. Mou, A. Li, H. Liu, Construction of titanium dioxide nanorod/graphite microfiber hybrid electrodes for a high performance electrochemical glucose biosensor, Nanoscale 8 (2016) 9382–9389. J. Zhang, A. Li, X. Yu, W. Guo, Z. Zhao, J. Qiu, X. Mou, J. Claverie, H. Liu, Scaly graphene oxide/graphite fiber hybrid electrodes for DNA biosensors, Adv. Mater. Interfaces 2 (2015) 1500072. M. Kang, Y. Lee, H. Jung, J. Shim, N. Lee, J. Baik, S. Lee, C. Lee, Y. Lee, M. Kim, Single carbon fiber decorated with RuO2 nanorods as a highly electrocatalytic sensing element, Anal. Chem. 84 (2012) 9485–9491. M. Zhang, K. Liu, L. Xiang, Y. Lin, L. Su, L. Mao, Carbon nanotube-modified carbon fiber microelectrodes for in vivo voltammetric measurement of ascorbic acid in rat brain, Anal. Chem. 79 (2007) 6559–6565. S. Ratha, C. Rout, Supercapacitor electrodes based on layered tungsten disulfidereduced graphene oxide hybrids synthesized by a facile hydrothermal method, ACS Appl. Mater. Interfaces 5 (2013) 11427–11433. N. Shelke, B. Karche, Hydrothermal synthesis of WS2/RGO sheet and their application in UV photodetector, J. Alloys Compd. 653 (2015) 298–303. J. Yang, D. Voiry, S. Ahn, D. Kang, A. Kim, M. Chhowalla, H. Shin, Two-dimensional hybrid nanosheets of tungsten disulfide and reduced graphene oxide as catalysts for enhanced hydrogen evolution, Angew. Chem. Int. Ed. 125 (2003) 13996–13999. B. Mahler, V. Hoepfner, K. Liao, G.A. Ozin, Colloidal synthesis of 1T-WS2 and 2HWS2 nanosheets: applications for photocatalytic hydrogen evolution, J. Am. Chem. Soc. 136 (2014) 14121–14127. D. Voiry, H. Yamaguchi, J. Li, R. Silva, D.C.B. Alves, T. Fujita, M. Chen, T. Asefa, V.B. Shenoy, G.E.M. Chhowalla, Enhanced catalytic activity in strained chemically exfoliated WS2 nanosheets for hydrogen evolution, Nat. Mater. 12 (2013) 850–855. A.A. Jeffery, C. Nethravathi, M. Rajamathi, Two-dimensional nanosheets and layered hybrids of MoS2 and WS2 through exfoliation of ammoniated MS2 (M = Mo, W), J. Phys. Chem. C 118 (2014) 1386–1396. X. Chia, A. Ambrosi, D. Sedmidubský, Z. Sofer, M. Pumera, Precise tuning of the charge transfer kinetics and catalytic properties of MoS2 materials via electrochemical methods, Chem. Eur. J. 20 (2014) 17426–17432.